Combined Modification of Fiber Materials by Enzymes and Metal Nanoparticles for Chemical and Biological Protection

To obtain fiber materials with pronounced chemical-biological protection, metal (Zn or Ta) nanoparticles were jointly applied with polyelectrolyte complexes of enzymes and polypeptides being their stabilizers. Computer modeling revealed the preferences between certain polyelectrolyte partners for N-acyl-homoserine lactone acylase and hexahistidine-tagged organophosphorus hydrolase (His6-OPH) possessing the quorum quenching (QQ) behavior with bacterial cells. The combinations of metal nanoparticles and enzymes appeared to function better as compared to the combinations of the same QQ-enzymes with antibiotics (polymyxins), making it possible to decrease the applied quantities by orders of magnitude while giving the same effect. The elimination of Gram-positive and Gram-negative bacterial cells from doubly modified fiber materials notably increased (up to 2.9-fold), whereas His6-OPH retained its hydrolytic activity in reaction with organophosphorus compounds (up to 74% of initially applied activity). Materials with the certain enzyme and Zn nanoparticles were more efficient against Bacillus subtilis cells (up to 2.1-fold), and Ta nanoparticles acted preferentially against Escherichia coli (up to 1.5-fold). Some materials were proved to be more suitable for combined modification by metal nanoparticles and His6-OPH complexes as antimicrobial protectants.


Introduction
Currently, chemical and biological safety still plays a huge role in human life in various military and peacetime operations, including chemical attacks, man-made disasters caused by the leakage of chemicals and biological agents, the use of pesticides in agriculture, contact with pathogenic microorganisms during the storage of agricultural products, etc. [1][2][3]. Most materials that can provide both chemical and biological defense to consumers are highly specialized, and their use is mostly limited to military and other special agencies. Thus, many people encountering dangerous agents on a daily basis are commonly unprotected.
The general approach to countering chemical and biological hazards is still isolation from them [4]. Meanwhile, there is a tremendous progress in the development of novel materials, especially nanomaterials [5], allowing not only prevention of their direct impact on humans, but also the active elimination of such biological pathogens and toxic chemical compounds [6]. Universal materials eliminating both chemical and biological hazards seem to be the most promising for application. In this vein, several approaches have been proposed, using: (i) inorganic metal nanoparticles (NPs), e.g., ZnO [7] and other metal oxides [8]; (ii) nanocomposites, e.g., Ag@Al 2 O 3 [9] and Ag@ZnTiO 3 [10]; (iii) enzymatic biocatalysts, e.g., combinations of horseradish peroxidase and glucose oxidase with chemically modified carriers [11]; etc. Such materials can be photoresponsive (i.e., have photocatalytic The lowest and highest binding energies (i.e., affinity) were estimated for PLD50 and PEG-PLE50, respectively ( Figure 2). Though there was a statistically significant difference in the means of affinity (according to one-way ANOVA, p = 0.007), only groups PLD50 vs. PEG-PLE50 and PLD50 vs. PEG-PLD50 differed enough (according to Holm-Sidak pairwise multiple comparison method, p = 0.017 and p = 0.022, respectively), while the other groups had no statistically significant difference.
The minimal and maximal areas were determined for PEG-PLE50 and succinylated gelatine (gelofusine), respectively ( Figure 2). Cumulatively, PLE50 was selected as a trade-off between the strength of complexing with enzyme and the possible negative influence on enzyme activity owing to occupation of enzymatic active site.
As compared to His6-OPH, there was a variability in affinity (e.g., in the case of PLD50) or in occupied area (e.g., in most cases, excepting PLE50 and PLD50). Thus, PLE50 could be a universal partner for both His6-OPH and PvdQ, and could possibly be approximated for other enzymes. Interestingly, only succinylated gelatin (gelofusine) appeared to be an absolutely poor partner for both enzymes.
Furthermore, complexes of PLE50 with PGA or His6-OPH and with additions of polymyxin B or polymyxin E (colistin) were issued towards Gram-positive bacteria Bacillus subtilis and Gram-negative bacteria Escherichia coli according to a previously developed method using bacterial cellulose [16] (Figure 3).
At neutral values of pH, the complexing of enzymes with both PLE50 and polymyxins had some effect on the antibacterial activity of the latter. These effects were minimal for His6-OPH vs. B. subtilis and for PGA vs. E. coli. Combined preparations based on His6-OPH showed more constant characteristics with polymyxin B, while PGA preferred combination with polymyxin E. The lowest and highest binding energies (i.e., affinity) were estimated for PLD 50 and PEG-PLE 50 , respectively ( Figure 2). Though there was a statistically significant difference in the means of affinity (according to one-way ANOVA, p = 0.007), only groups PLD 50 vs. PEG-PLE 50 and PLD 50 vs. PEG-PLD 50 differed enough (according to Holm-Sidak pairwise multiple comparison method, p = 0.017 and p = 0.022, respectively), while the other groups had no statistically significant difference.
The minimal and maximal areas were determined for PEG-PLE 50 and succinylated gelatine (gelofusine), respectively ( Figure 2). Cumulatively, PLE 50 was selected as a tradeoff between the strength of complexing with enzyme and the possible negative influence on enzyme activity owing to occupation of enzymatic active site.
As compared to His 6 -OPH, there was a variability in affinity (e.g., in the case of PLD 50 ) or in occupied area (e.g., in most cases, excepting PLE 50 and PLD 50 ). Thus, PLE 50 could be a universal partner for both His 6 -OPH and PvdQ, and could possibly be approximated for other enzymes. Interestingly, only succinylated gelatin (gelofusine) appeared to be an absolutely poor partner for both enzymes.
Furthermore, complexes of PLE 50 with PGA or His 6 -OPH and with additions of polymyxin B or polymyxin E (colistin) were issued towards Gram-positive bacteria Bacillus subtilis and Gram-negative bacteria Escherichia coli according to a previously developed method using bacterial cellulose [16] (Figure 3).
At neutral values of pH, the complexing of enzymes with both PLE 50 and polymyxins had some effect on the antibacterial activity of the latter. These effects were minimal for His 6 -OPH vs. B. subtilis and for PGA vs. E. coli. Combined preparations based on His 6 -OPH showed more constant characteristics with polymyxin B, while PGA preferred combination with polymyxin E.  to bacterial cellulose treated with polymyxin B or polymyxin E, enzymes (His6-OPH or PGA), or their combinations. ATP of bacterial cells similarly exposed on the same bacterial cellulose with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a PBS buffer (pH 7.4), and enzymes were additionally stabilized in complexes with PLE50. Designation: ○-control without enzyme, ✩-with PGA, ▲-with His6-OPH, w/o-without polymyxins.

Combination of Metal Nanoparticles with Enzymes within Fiber Materials
Initially, the kinetics of bacterial elimination was investigated for materials modified by Ta NPs and complexes of His6-OPH with PEG-PLE50 obtained at pH 10.5 (i.e., pH-optimum of the enzyme) ( Figure 4). Such complexes of His6-OPH with PEG-PLE50 have previously been shown to provide maximum stabilization under harsher conditions [21].   , or their combinations. ATP of bacterial cells similarly exposed on the same bacterial cellulose with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a PBS buffer (pH 7.4), and enzymes were additionally stabilized in complexes with PLE50. Designation: ○-control without enzyme, ✩-with PGA, ▲-with His6-OPH, w/o-without polymyxins.

Combination of Metal Nanoparticles with Enzymes within Fiber Materials
Initially, the kinetics of bacterial elimination was investigated for materials modified by Ta NPs and complexes of His6-OPH with PEG-PLE50 obtained at pH 10.5 (i.e., pH-optimum of the enzyme) ( Figure 4). Such complexes of His6-OPH with PEG-PLE50 have previously been shown to provide maximum stabilization under harsher conditions [21]. and E. coli bacterial cells (B) exposed for 24 h to bacterial cellulose treated with polymyxin B or polymyxin E, enzymes (His 6 -OPH or PGA), or their combinations. ATP of bacterial cells similarly exposed on the same bacterial cellulose with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a PBS buffer (pH 7.4), and enzymes were additionally stabilized in complexes with PLE 50 . Designation: -control without enzyme, Int. J. Mol. Sci. 2022, 23, 1359 8 of 15 similarly exposed on the same materials with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a PBS buffer (pH 7.4). Designation: •-polymyxin, ×-PGA, ∆-His6-OPH, ✩ -PGA with polymyxin, ▲-His6-OPH with polymyxin.
As opposed to bacterial cellulose, the structure of fiber material significantly influenced the efficiency of the polymyxins and their combinations with enzymes. The highest synergic effect at pH 7.4 towards B. subtilis ( Figure 6) was found in combination of polymyxin E with PGA loaded onto materials #1 and #3, while towards E. coli it was for the same enzyme on material #4. The His6-OPH was in the middle, though it slightly preferred material #2 and polymyxin B.
The picture changed drastically when pH was increased to 9.5 ( Figure 7). The combination of polymyxin B with His6-OPH became the absolute leader towards both B. subtilis and E. coli, irrespective of the material used. PGA showed comparable efficiency only with polymyxin E on materials #1, #2 and #3 towards B. subtilis, with polymyxin B on materials #2, #3 and #4 towards E. coli, or with polymyxin E on materials #1, #2 and #4 towards E. coli.

Combination of Metal Nanoparticles with Enzymes within Fiber Materials
Initially, the kinetics of bacterial elimination was investigated for materials modified by Ta NPs and complexes of His 6 -OPH with PEG-PLE 50 obtained at pH 10.5 (i.e., pH-optimum of the enzyme) ( Figure 4). Such complexes of His 6 -OPH with PEG-PLE 50 have previously been shown to provide maximum stabilization under harsher conditions [21].  Viable cells gradually decreased over time in all variants. However, Ta NPs alone or in combination with His 6 -OPH significantly increased the rate of cell death. The highest degree of cell death at 24 h exposure on materials #1, #2 and #3 was in the case of combination with His 6 -OPH, irrespective of the metal NPs used (Ta or Zn) ( Figure S1). The highest efficiency towards both microorganisms was revealed for combination with Ta NPs on materials #1, #2 and #3.
Further both PGA and His 6 -OPH complexes were similarly obtained and tested under the same conditions at pH 9.5 (i.e., intermediate value between the pH-optima of these enzymes) ( Figure 5). As previously, combinations with enzymes appeared to be preferable for metal NPs alone, while both enzymes in combination were almost undistinguishable between each other. Viable cells gradually decreased over time in all variants. However, Ta NPs alone or in combination with His6-OPH significantly increased the rate of cell death. The highest degree of cell death at 24 h exposure on materials #1, #2 and #3 was in the case of combination with His6-OPH, irrespective of the metal NPs used (Ta or Zn) ( Figure S1). The highest efficiency towards both microorganisms was revealed for combination with Ta NPs on materials #1, #2 and #3.
Further both PGA and His6-OPH complexes were similarly obtained and tested under the same conditions at pH 9.5 (i.e., intermediate value between the pH-optima of these enzymes) ( Figure 5). As previously, combinations with enzymes appeared to be preferable for metal NPs alone, while both enzymes in combination were almost undistinguishable between each other. , enzymes (His6-OPH or PGA), or their combinations. ATP of bacterial cells similarly exposed on the same materials with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a Na-carbonate buffer (pH 9.5) and enzymes were additionally stabilized in complexes Interestingly, combinations with metal NPs seem to have variable specificity towards microorganisms, and as a result, combinations with Zn and Ta were most effective towards B. subtilis and E. coli cells, respectively. The antimicrobial activity of materials #1, #3 and #4 appeared to be slightly more pronounced towards B. subtilis, and materials #1, -Ta NPs with PGA, -Ta NPs with His 6 -OPH.
Interestingly, combinations with metal NPs seem to have variable specificity towards microorganisms, and as a result, combinations with Zn and Ta were most effective towards B. subtilis and E. coli cells, respectively. The antimicrobial activity of materials #1, #3 and #4 appeared to be slightly more pronounced towards B. subtilis, and materials #1, #2 and #3 were more effective towards E. coli.

Combination of Polymyxins with Enzymes within Fiber Materials
To reveal the applicability of the procedure, conventional antibiotics were applied in combination with enzymes to fiber materials under the same protocol (Figures 6 and 7). Interestingly, combinations with metal NPs seem to have variable specificity towards microorganisms, and as a result, combinations with Zn and Ta were most effective towards B. subtilis and E. coli cells, respectively. The antimicrobial activity of materials #1, #3 and #4 appeared to be slightly more pronounced towards B. subtilis, and materials #1, #2 and #3 were more effective towards E. coli.

Combination of Polymyxins with Enzymes within Fiber Materials
To reveal the applicability of the procedure, conventional antibiotics were applied in combination with enzymes to fiber materials under the same protocol (Figures 6 and 7).  As opposed to bacterial cellulose, the structure of fiber material significantly influenced the efficiency of the polymyxins and their combinations with enzymes. The highest synergic effect at pH 7.4 towards B. subtilis (Figure 6) was found in combination of polymyxin E with PGA loaded onto materials #1 and #3, while towards E. coli it was for the -PGA with polymyxin, -His 6 -OPH with polymyxin. same enzyme on material #4. The His6-OPH was in the middle, though it slightly preferred material #2 and polymyxin B.
The picture changed drastically when pH was increased to 9.5 ( Figure 7). The combination of polymyxin B with His6-OPH became the absolute leader towards both B. subtilis and E. coli, irrespective of the material used. PGA showed comparable efficiency only with polymyxin E on materials #1, #2 and #3 towards B. subtilis, with polymyxin B on materials #2, #3 and #4 towards E. coli, or with polymyxin E on materials #1, #2 and #4 towards E. coli. or polymyxin E (C,D), enzymes (His 6 -OPH or PGA), or their combinations. ATP of bacterial cells similarly exposed on the same materials with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a Na-carbonate buffer (pH 9.5) and enzymes were additionally stabilized in complexes with PLE 50 . Designation: •-polymyxin, ×-PGA, ∆-His 6 -OPH, As opposed to bacterial cellulose, the structure of fiber material significantly influenced the efficiency of the polymyxins and their combinations with enzymes. The highest synergic effect at pH 7.4 towards B. subtilis ( Figure 6) was found in combination of polymyxin E with PGA loaded onto materials #1 and #3, while towards E. coli it was for the same enzyme on material #4. The His 6 -OPH was in the middle, though it slightly preferred material #2 and polymyxin B.
The picture changed drastically when pH was increased to 9.5 ( Figure 7). The combination of polymyxin B with His 6 -OPH became the absolute leader towards both B. subtilis and E. coli, irrespective of the material used. PGA showed comparable efficiency only with polymyxin E on materials #1, #2 and #3 towards B. subtilis, with polymyxin B on materials #2, #3 and #4 towards E. coli, or with polymyxin E on materials #1, #2 and #4 towards E. coli.

Activity of His 6 -OPH within Modified Fiber Materials
Activity of His 6 -OPH within modified fiber materials was investigated with a paraoxon as substrate at pH 10.5 (Figure 8). A lot of enzyme activity was retained within materials #2, #3 and #4. It was maximal with Ta NPs, and especially on material #3. However, enzyme activity was dramatically reduced on the 2nd and subsequent application cycles. The best retention of activity was observed during the 2nd and subsequent repeated uses of material #2, irrespective of the applied metal NPs. polymyxin E (C,D), enzymes (His6-OPH or PGA), or their combinations. ATP of bacterial cells similarly exposed on the same materials with treatment by buffer (i.e., controls) was taken as 100%. All solutions were prepared in a Na-carbonate buffer (pH 9.5) and enzymes were additionally stabilized in complexes with PLE50. Designation: •-polymyxin, ×-PGA, ∆-His6-OPH, ✩ -PGA with polymyxin, ▲-His6-OPH with polymyxin.

Activity of His6-OPH within Modified Fiber Materials
Activity of His6-OPH within modified fiber materials was investigated with a paraoxon as substrate at pH 10.5 (Figure 8). A lot of enzyme activity was retained within materials #2, #3 and #4. It was maximal with Ta NPs, and especially on material #3. However, enzyme activity was dramatically reduced on the 2nd and subsequent application cycles. The best retention of activity was observed during the 2nd and subsequent repeated uses of material #2, irrespective of the applied metal NPs. Figure 8. Residual activity of His6-OPH loaded onto multiple fiber materials (#1, #2, #3, and #4) treated with Zn (A) or Ta NPs (B) during repeated application. Initial loaded activity of His6-OPH (1 U) was taken as 100%. The His6-OPH was prepared as a complex with PEG-PLE50 in a Na-carbonate buffer (pH 10.5). Absent columns indicate that residual activity was equal to or less than limit of determination (0.01 U).

Discussion
The formation of enzyme-polyelectolyte complexes makes it possible to significantly stabilize enzymes in harsh environmental conditions [17,[19][20][21]. Since protective materials are supposed to be applied under such conditions, the enzymes within them have to be stabilized somehow. Though such stabilized preparations of His6-OPH have been developed already, complexes for an alternative enzyme-PGA-were designed in the current work for the first time. Despite this not being the main purpose of the work, complexes of PGA with PLE50 appeared to be quite useful and could be interesting. Namely, the lowest affinity for PLD50 could result in too strong binding of polymer to enzyme, and thus in losses of activity due to hindrances to structural mobility. On the other hand, the highest affinities being observed for PEGylated polypeptides, especially PEG-PLE50, are likely to lead to unstable complexes, and thus to lower enzyme stabilization. Succinylated gelatin (gelofusine) had comparable affinity with PLE50 but also occupied too much area on the enzyme surface, which could also result in activity loss [20]. Thus, PLE50 is a consensus polymer and also applicable with His6-OPH.
At present, there are several major paradigms of formation of stable/resistant microbial communities and their destruction by action of organic and inorganic active compounds [22]. In this continuum, enzymes (like PGA or His6-OPH) are supposed to intercept and destroy simple molecular messengers used by bacteria in their interaction in the so-called Quorum Figure 8. Residual activity of His 6 -OPH loaded onto multiple fiber materials (#1, #2, #3, and #4) treated with Zn (A) or Ta NPs (B) during repeated application. Initial loaded activity of His 6 -OPH (1 U) was taken as 100%. The His 6 -OPH was prepared as a complex with PEG-PLE 50 in a Nacarbonate buffer (pH 10.5). Absent columns indicate that residual activity was equal to or less than limit of determination (0.01 U).

Discussion
The formation of enzyme-polyelectolyte complexes makes it possible to significantly stabilize enzymes in harsh environmental conditions [17,[19][20][21]. Since protective materials are supposed to be applied under such conditions, the enzymes within them have to be stabilized somehow. Though such stabilized preparations of His 6 -OPH have been developed already, complexes for an alternative enzyme-PGA-were designed in the current work for the first time. Despite this not being the main purpose of the work, complexes of PGA with PLE 50 appeared to be quite useful and could be interesting. Namely, the lowest affinity for PLD 50 could result in too strong binding of polymer to enzyme, and thus in losses of activity due to hindrances to structural mobility. On the other hand, the highest affinities being observed for PEGylated polypeptides, especially PEG-PLE 50 , are likely to lead to unstable complexes, and thus to lower enzyme stabilization. Succinylated gelatin (gelofusine) had comparable affinity with PLE 50 but also occupied too much area on the enzyme surface, which could also result in activity loss [20]. Thus, PLE 50 is a consensus polymer and also applicable with His 6 -OPH.
At present, there are several major paradigms of formation of stable/resistant microbial communities and their destruction by action of organic and inorganic active compounds [22]. In this continuum, enzymes (like PGA or His 6 -OPH) are supposed to intercept and destroy simple molecular messengers used by bacteria in their interaction in the socalled Quorum Sensing (QS) state [23]. Namely, both PGA and His 6 -OPH hydrolyze N-acyl homoserine lactones (AHLs) of some Gram-negative bacteria. Both Gram-positive B. subtilis and Gram-negative E. coli cells are not known to use any AHLs in their QS. This raises a question as to how it is possible that PGA and His 6 -OPH have any positive effect in the current experimental design with antibacterials of two different modalities (i.e., NPs and polymyxins). Hypothetically, for these enzymes there can be other metabolic targets that play important role within cells. Otherwise, bacteria may shift their metabolome during QS and the subsequent colonization of the fiber materials and bacterial cellulose, with the enzymes acting on metabolites other than AHLs. Yet another option, proposed previously [15], is that enzymes act as a 'shuttle' for antibacterials to penetrate into bacterial cells. Currently, it is not possible to make a certain conclusion as to the mechanism of the observed effects. However, further studies are required to elucidate these results.
From a practical standpoint, combinations of metal NPs with enzymes seem preferable to combinations of the same enzymes with polymyxins. Firstly, the quantities of NPs required to achieve a similar effect were 5.6 and 21.7 times lower (for Zn and Ta NPs, respectively). For example, less than 5 mg of Ta NPs was applied per 1 m 2 . Secondly, it looks like these NPs did not show any preferences for an enzyme to combine with. Thirdly, the antibiotics used in this work are for medical application, and thus their 'improper' usage could intensify development of resistance to these antibiotics in microorganisms.
An EC 50 dosage applied to materials in combination with enzymes resulted in an improvement up to EC 80 for most of the fibers. However, little individual specificity of the combined modification to different bacterial cells was revealed, and materials based on Zn and Ta NPs seemed to be slightly preferable for eliminating B. subtilis and E. coli cells, respectively. Currently, it is not possible to directly compare the obtained materials with other examples known from the literature, due to several reasons. Firstly, most authors have used the agar plate antibacterial test (i.e., leaching of nanomaterials) or, much more rarely, the broth test (i.e., immersion of fibers into medium with subsequent leaching of nanomaterials). They are both difficult to apply for the testing of personal protective equipment. Secondly, the content of nanomaterials (if there is any) is larger by orders of magnitude in comparison to the current work, for example, it was at least 200 mg/m 2 ZnO NPs in [7]; up to 14 g/m 2 Ag and up to 69 g/m 2 ZnTiO 3 NPs in [10]; 11.5 wt.% Ag@TiO2 nanocomposite in [12]; or even cannot be estimated without additional data, as in the case of [9,13].
The fiber materials which were applied as a base also varied to a great extent: nylon 6 [7]; poly(vinylidene difluoride) [9]; multilayer composite (mostly unspecified, excepting layers of polyethylene terephthalate and of activated carbon) [10]; polyurethane [12]; and activated carbon fibers [13]. Additional dimethylacrylamide-methacrylate copolymer was revealed when investigating an 'enzyme only' material [11]. Proper selection of the base material was shown in the current work to influence antibacterial and enzyme activity significantly. In summary, materials #2 and #3, both containing polyester (more probably polyethylene terephthalate), appear to be the most suitable for combined modification with metal NPs and His 6 -OPH complexes. Although material #1 showed good antibacterial activity with both NPs and antibiotics, and had similar composition as #3 but a 1.7-fold lower surface density, it exhibited poor retention of His 6 -OPH complexes (Figure 8).
Despite positive results in genere, there are still some problems. Namely, His 6 -OPH seems to be actively eluted from all fiber materials (Figure 8). This process is highly likely to occur simultaneously with elution of metal NPs. In this work, they were simply adsorbed onto the fiber materials, and could be easily desorbed. To prevent such excessive losses, preliminary chemical and/or physical modification of such fibers could be helpful.

Materials
Polymyxin B, polymyxin E (=colistin), penicillin G acylase (PGA) from E.coli and paraoxon (diethyl 4-nitrophenyl phosphate) were purchased from Sigma-Aldrich (Darmstadt, Germany). Polyglutamic acid (PLE 50 ) and pegylated PLE 50 (PEG-PLE 50 ) were obtained from Alamanda Polymers (Huntsville, AL, USA). Recombinant E. coli strain SG13009[pREP4] (Qiagen, Hilden, Germany) transformed by a plasmid encoding His 6 -OPH was used for the production of His 6 -OPH by a patented method and, further, the enzyme was purified by a published procedure [24]. According to methods described earlier [25], His 6 -OPH concentration was determined by Bradford assay with Coomassie Brilliant Blue G-250 (Sigma-Aldrich); protein purity was analyzed by sodium dodecyl sulfate polyacrylamide gel electrophoresis in a 12% polyacrylamide gel using a Mini-PROTEAN II cell (Bio-Rad, Hercules, CA, USA) followed by Coomassie Brilliant Blue R-250 (Sigma-Aldrich) staining, and was ca. 98 ± 0.5%. Enzyme-polyelectrolyte complexes were obtained by previously published method [20,21] by simple mixing of an enzyme and polymer solution at molar ratio 1:1.
Bacterial cellulose was produced with Komagataeibacter xylinum B-12429 cells, as previously described for a medium with fructose [26,27], then dried at room temperature overnight under sterile conditions and cut to samples of 1 × 1 cm before further use.

Preparation and Characterization of Metal Nanoparticles
Metal NPs were obtained in a plasma electric arc discharge as published previously [14,28] using ethanol as a solvent. They were characterized by size using a transmission electron microscope LEO 912 AB OMEGA (Carl Zeiss, Oberkochen, Germany) with energy filter and Keller system; by size distribution and ζ-potential using dynamic light scattering on a Zetasizer Nano ZS (Malvern Instruments, Worcestershire, UK); by qualitative elemental composition using an atomic-emission spectrometer iCAP 6300 Radial View (Thermo Fisher Scientific Inc., Waltham, MA, USA) with inductively coupled plasma.

Preparation and Antibacterial Activity of Modified Bacterial Cellulose (BC)
All tested BC samples loaded by antimicrobial agents and hydrolytic enzymes were prepared by the same general procedure [16] with minor modifications. To wit, 10 µL of 10 g/L antimicrobial agent and 5 µL of 2.5 g/L PGA (or 1 g/L His 6 -OPH) complexed with PLE 50 (at molar ratio 1:1) in a PBS buffer (pH 7.4) were sequentially applied to samples of bacterial cellulose (1 cm × 1 cm) and dried for 20-22 h at +8 • C under sterile conditions. Then, antibacterial activity was analyzed according to the previously published procedure [14] with cells of the G(−) bacterium E. coli DH5α (Thermo Fisher Scientific, Waltham, MA, USA), and the G(+) bacterium B. subtilis B-522 (All-Russian Collection of Microorganisms, Russia). Cells were aerobically cultivated in Luria-Bertani (LB) culture medium on a thermostatically controlled Adolf Kuhner AG shaker (Basel, Switzerland) at 37 • C and agitation of 150 rpm. Cell growth was monitored with an Agilent UV-8453 spectrophotometer (Agilent Technology, Waldbronn, Germany) at 540 nm. Bacterial cells were grown for 18-20 h, and then separated from the culture broth by centrifugation at 8000× g for 10 min (Avanti J25, Beckman, Brea, CA, USA). Cell biomass was suspended in a sterile 0.9% NaCl solution and 20 µL of suspension with cells concentration of (2 ± 0.5) × 10 6 cells/mL was loaded onto the BC samples. After 24 h of exposure, samples were placed in 1 mL of DMSO and gently stirred. Following 3 h of extraction, the residual concentration of ATP in the extract was determined using a standard luciferin-luciferase ATP reagent (Lyumtek Ltd., Moscow, Russia) by a known protocol [29,30]. BC samples containing only individual antimicrobial agents (i.e., polymyxin B or colistin) without enzymes were used as positive controls, while BC samples similarly treated with PBS buffer only were used as negative controls. The intensity of bioluminescence was measured using a Microluminometer 3560 (New Horizons Diagnostic, Arbutus, MD, USA). The calibration curves for the determination of cell concentrations were plotted, where the concentration of ATP was used as a function of the concentration of colony-forming units (CFU), calculated by a traditional microbiological method, using agar-containing media.
The effective concentrations of antimicrobials leading to a 50% decrease in the amount of living cells were assumed as values of EC 50 . The experiments were undertaken no less than in triplicate.

Preparation and Antibacterial Activity of Modified Fibrous Materials
Metal NPs were deposited onto fibrous materials as described previously [14], with minor modifications. Briefly, 25 µL of 18.3 mg/L Ta (or 71.7 mg/L Zn) NPs in ethanol were dropwise loaded per sample (1 × 1 cm) and then dried overnight at a room temperature within Petri dishes. Then, 5 µL of 0.3 g/L His 6 -OPH (or 0.5 g/L PGA) complexed with PLE 50 in a PBS buffer (pH 7.4) or Na-carbonate buffer (pH 9.5) were applied and dried for 20-22 h at +8 • C under sterile conditions. After that, antibacterial activity was determined as described above for BC. Samples treated with both NPs and buffers were used as positive controls, while samples similarly treated only with buffers were used as negative controls.
Analogously, conventional antimicrobial agents (polymyxin B and colistin) were tried for fibrous materials modification. Five microliters of 2 g/L antimicrobial agent and 0.3 g/L His 6 -OPH (or 0.5 g/L PGA) complexed with PLE 50 in a PBS buffer (pH 7.4) or Na-carbonate buffer (pH 9.5) were applied to samples (1 × 1 cm) and dried for 20-22 h at +8 • C under sterile conditions. Then, antibacterial activity was determined, while similar controls were issued.
To investigate the kinetics of cell death, a special series of samples modified by Ta (or Zn) NPs and His 6 -OPH (in complex with PEG-PLE 50 in Na-carbonate buffer, pH 10.5) was prepared as described above. Bacterial suspension was loaded shortly (i.e., at t = 0). After that, samples were withdrawn individually at certain time points of exposure and analyzed.

Hydrolytic Activity of Modified Fibrous Materials
Dried samples of fibrous materials modified by Ta (or Zn) NPs and 1 U of His 6 -OPH (in complex with PEG-PLE 50 in Na-carbonate buffer, pH 10.5) were placed in a stirred vessel with 1.8 mL of Na-carbonate buffer (pH 10.5). Then, 0.2 mL of 10 mM paraoxon water solution was added, and the kinetics of the product (4-nitrophenol) growth was monitored for 5 min by sampling a 0.1 mL of a reaction medium into 0.9 mL of the same buffer and measuring OD with an Agilent UV-8453 spectrophotometer at 405 nm. After that, a reaction medium was decanted, and samples were gently washed once with 2 mL of the buffer before further use. Similar samples without His 6 -OPH were applied analogously and used as controls. The initial linear parts of kinetic curves (V o = tg α) were used to calculate enzymatic activity of modified fiber materials. One unit of enzyme activity was defined as the quantity of the enzyme necessary to hydrolyse 1 µmol of paraoxon per min at 25 • C.

Computational Methods
Crystallographic structure of PvdQ from Pseudomonas aeruginosa was obtained from the Protein Data Bank (PDB 4M1J).
Simulations of enzyme-ligand complexes were performed at the Supercomputing Center of Lomonosov Moscow State University [34], using up to 512 cores of Intel Xeon X5570 2.93GHz and 1.5 TB of memory. For that, AutoDock Vina (ver. 1.1.2, available at http://vina.scripps.edu/, accessed on 25 January 2022) [35] with Intel MPI Library (ver. 5.0.1) was applied with default program options as published earlier [20]. The grid box was approximately centered on the center of mass of the enzyme and its size was chosen so that enzyme molecule was within the box plus an additional margin. Following the procedure, the "receptor" (i.e., enzyme) was proposed as rigid and the "ligand" (i.e., polymer) was fully flexible. Results were visually inspected for possible errors or molecular intersections, and six poses with minimal energy were selected.
The solvent-accessible area occupied by polymers on the surface of the enzyme was calculated using the "get_area" function of PyMOL Molecular Graphics System (ver. 1.7.6, Schrödinger Inc., New York, NY, USA). Statistical analysis was realized using SigmaPlot (ver. 12.5, Systat Software Inc., San Jose, CA, USA) and OriginPro (ver. 9.4.2, OriginLab Corporation, Northampton, MA, USA), and the data are presented as means ± standard deviation (± SD) unless otherwise stated.

Conclusions
Thus, novel fiber materials of double functionality were successfully obtained in the work via a simple procedure. Up-to-date methods from nanotechnology and biotechnology were combined to produce highly effective materials. The prospectively suggested approach may make it possible to greatly expand the spectrum of the toxic compounds that can be eliminated chemically and/or enzymatically by such protective materials. Namely, the target toxins may be (but not limited to) those produced biologically (like mycotoxins, bacterial toxins, venoms, etc.) and antropogenically (like gases, vapours, solubles, etc.).

Conflicts of Interest:
The authors declare no conflict of interest. I.L., N.S. and E.E. are named coinventors of several Russian patents that involve organophosphorus hydrolase and its modified forms as a base active compound. The funders had no role in the design of the study; in the collection, analyses, or interpretation of data; in the writing of the manuscript, or in the decision to publish the results.